Micromeso draping modelling of noncrimp fabrics


 Bridget Mary Howard
 1 years ago
 Views:
Transcription
1 Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are widely used in the composite materials as a reinforcement part due to a combination of both high mechanical properties in main fibre directions and better handling compared to UD tapes. For prediction of mechanical response of composite parts in particular with high curvature it is important to consider the local orientations and gaps in textile structures obtained after draping. For this goal the simulations on the textile structure scale (mesoscale) are commonly used. In the present work the new approach for the modelling of the textile structures is proposed. In this approach the mechanical properties of the textile yarns are obtained from the microscale simulations of the glass roving. This allows to investigate the dependency to the fibre volume fraction (FVFr) of the roving. Although microscale modelling as the basis for textile simulations was used in [1], but only small micromodels without taking into account the crosssection change during the compaction was investigated. Latter can play a major role in forming processes like RTM. The representative volume element (RVE) of the structure should be generated without the interpenetrations, which is hardly possible for geometrical generation especially for the complex textile structures such as NCFs [2]. New method for the generating of the free of interpenetrations RVE based on the thermal expansion in transverse direction was proposed. The other aspect of the composite simulations is the prediction of the mechanical properties. Commonly used method where the textile geometry is subtracted from the matrix is causes bad quality mesh of the model or fails at all. For this reason the mesh superposition (MSP) [3, 4] technique is preferable for investigating of the stiffness behaviour. In present work this was implemented in LS Dyna. 2 Micromodelling of the roving Generally the roving can be described as a transverse isotropic material with axis of symmetry on the roving length axis. There are six main deformation modes: length tension and compaction, transverse tension and compaction, shear and torsion. In this work following assumptions are made:  compression stiffness in length direction as well as tension stiffness in transverse direction of the roving is negligible;  length stiffness of the roving has a linear dependency only on FVFr and may be calculated due to mixture rule like E E is a filament elastic modulus;, where is the FVFr and l f l E l f  there is no significant strain in transverse direction due to length deformation, so the poisson s ratio ; lt  fibrefibre friction is assumed to be constant. The constitutive law of the roving material in this case may be written as follows: x 1 E l f x y 1 Et tt Et y z tt Et 1 Et z xy 1 2Gtl xy yz 1 2Gtt yz G 1 2 xz tl xz This means that we need to define four constants that should depend nonlinear on the FVFr θ. 2.1 Used models For determination of the missing mechanical properties, quasistatic FE simulations on microscale were performed. Used models for different load cases are presented on the Figure 1. (1)
2 Fig.1: Roving models used for microsimulations: (a) transverse compaction, (b) torsion and (c) shear loading cases. The mechanical properties of the filaments were taken from the data sheet of the glass roving, which was used for manufacturing of the lenowoven NCFs. The diameter of one filament is 17m, density g cm, isotropic elastic modulus E f 82GPa with poisson s ratio. 2 f d f. Friction coefficient for fibrefibre contact was chosen to be.3. The filaments in the roving have some degree of misalignment due to the manufacturing processes of the textile and roving itself. In this work this effect was investigated by performing the simulations for various standard deviations of the filament angle. The structures were generated with GeoDict software [5] and then these models were transferred to LSDyna a converter software with developed in FTA [6]. These models have about 6 filaments inside of the domain of 1x.5x.5 mm³ for dom x, dom y and dom z respectively. Initial FVFr of the models was about 25% depending on the standard deviation of the filament orientations. To ensure the contact, each filament is represented as a sequence of HighLiu beams with length of l 2 d 34m. Rigid walls (RW) are generated on the sides of the domain. Periodicity in length f b f direction was implemented through restriction of displacement in xdirections as well as rotations along y and z axis for nodes, that lie on the domain x face. 2.2 Transverse compaction The general model for transverse compaction is represented at Figure 1 a. The roving is compressed in z direction so as the final FVFr would be. 85. f The upper RW z compresses the roving, while other three remain stationary. This approach allows to investigate on one loading case both the compression stiffness and the expansion effect in other transverse direction (y), which is nonlinear and may be significant for higher FVFrs. The pressure versus FVFr dependency for both z and y directions is shown in Figure 2. It may be seen, that the basic shape of the curves remains the same with shifting to small FVFr when the filament misalignment increases. Both y and z pressures start to increase at the same FVFr. f
3 Fig.2: Pressure in compression and transverse directions of the roving on microscale for different standard deviations of the filaments orientations. Further, the poisson s ratio and transverse elastic modulus may be expressed through the RW pressure values as follows: P P ; E P P, (2) tt y z t z tt y z where z is the logarithmic strain in compaction direction. Fig.3: Elastic modulus and poisson s coefficient of the roving on microscale for different standard deviations of the filaments orientations. The shape of the E comp curve remains smooth, while the poisson s tends to oscillate (Figure 3). It can be solved by using the models with higher amount of filaments inside and thus bigger domain dimansions. Still with used models the general trends of increasing of the poisson s ratio with increasing of the FVFr. The slope of the curve decreases with increasing of the filament misalignment. Model results were written out during the solution for FVFr of.5,.6,.7 and.8 for further torsion and shear calculations. 2.3 Torsion The torsion of 1 is applied to the roving as shown on the Figure 1 b. The shear modulus is then computed as follows: where inertia. G 2 E dom J int 2 x tt, (3) E int is the internal energy of the roving,  torsion angle and J is a polar area moment of
4 Results for different FVFr and filament misalignments with standard deviation of 1 and 4 are presented in the Figure 4. It may be seen, that with increasing of the FVFr and torsion angle the shear modulus in the ttplane increases. Fig.4: Shear modulus G tt versus torsion angle for a) 1 standard deviation of the filament orientation and b) Shear For the same models the shear simulations for determination of the shear modulus G lt were performed (Figure 1 c). Obtained shear modulus for standard deviation of 1 and 4 are represented in the Figure 5. Fig.5: Shear modulus G lt versus shear angle for a) 1 standard deviation of the filament orientation and b) 4. In this case it may be seen, that the shear modulus G lt doesn t change with the shear angle. As well as the trend to decreasing of the stiffness with increasing of the FVFr may be observed. This effect should be investigated in further studies. 3 Implementation of user defined material model The FVFr of the element may be obtained at each iteration as follows: exp, (4) t exp where is the initial FVFr of the element and 2 and 3 are the complete strains in the 2 and 3 directions respectively. The elastic modulus obtained from microscale simulation may be approximated with the power law as described in [1]. The poisson s ratio is also assumed to be approximated with power law. The shear modules are linear dependent from the FVFr: 2 3
5 B B E Et AE tt A ; Gtt At Bt ; Glt Al ; B, (5) where the A and B are constants for different mechanical properties obtained from the microsimulations of the roving. 4 Generation of the RVEs For the generation of the RVE the thermal expansion in the transverse direction of the rovings was used. It allows generating the complex textile structures without interpenetrations and use them for various simulations. The user defined material model described above was assigned to yarns. This allows to consider the local FVFr and real compression / shear behaviour. The dirichlet periodic boundary conditions (BC) were applied to the ends of the each yarn to estimate the periodicity of the obtained structure. Although the length of the auxiliary yarns was taken from the measurements on the real textile. Different RVE should be used for draping and mechanical simulations. From one hand, in the draping simulations the big areas of the textile should be modelled, so the model simplification plays very important role. The auxiliary yarns may be represented as beam elements and only two solid elements in thickness directions of the reinforcement yarns should be used. On the other hand, in mechanical simulations also the stress distributions inside of the auxiliary yarns and close to them may play a role, so more refined RVE is preferable. For this case the true shape of the yarns should be considered. 4.1 Draping simulation The initial textile structure with rescaled crosssections of the yarns is shown in the Figure 6. The auxiliary yarns in the initial condition have the circle crosssection and for preserving of the crosssection change during the thermal expansion simulation, the material MAT_22 was used with high transverse and length modules ( E1 E2 E3 ) but remaining the shear modules on the roving level. Different scale factors ( sf d init d real ) were used. l Fig.6: RVE of the lenowoven NCF for draping simulation: a) initial conditions, b) after thermal expansion simulation with calculated local FVFrs and c) auxiliary yarns are represented as beams. Obtained structure consists only of 112 solid elements and 6 beam elements with dimensions of RVE 4 x 4 cm². 4.2 Calculation of the mechanical properties In real structure the auxiliary yarns have an elliptical crosssection. This should be considered in the initial configuration, what yields to smaller initial crosssections. For obtaining the desired composite thickness, the rigid walls on the top and the bottom of the structure are generated (Figure 7).
6 Fig.7: RVE of the lenowoven NCF for calculation of the mechanical properties: a) initial conditions, b) after thermal expansion simulation with calculated local FVFrs. The crosssection of the generated structure conforms to the microcut image of real textile like shown in the Figure 8. Fig.8: Microcut image of the glass lenowoven NCF composite (a) and comparison with the simulation section view (b). 5 Validation of the developed model 5.1 Single roving compaction For validation purposes, the following experiment setup was used (Figure 9 a). It consists of two plates with the lower one is made of transparent material. A camera is located underneath, which is needed to record the width change during the compaction.
7 Fig.9: Roving compaction: a) experimental stand, b) roving outer surface. For estimation of the required parameters of the developed material model, the filament orientation distribution is necessary. For this purpose the outer surface of rovings taken from lenowoven NCF was microscopically investigated and the mean and standard deviation values were calculated (Figure 9 b). For this structure the average standard deviation value of the filament misalignment was The values of the transverse compaction elastic modulus and poisson s ratio were averaged between 5 and 6. The approximation with a power function is shown in Figure 1. Fig.1: Material parameters used for roving simulations: a) elastic modulus and b) poisson s ratio. The simulation results are showing good agreement with experimental results without some extra tuning of the parameters as it is shown on the Figure 11. Although some small deviations may be observed. These may be the reason of using relative small models for microsimulations as discussed above.
8 Fig.11: Comparison of the experimental and simulation results for roving compaction: a) compaction force per unit length and b) roving width versus roving thickness. 5.2 Stiffness of the composite The RVE described in Section 4.2 was used for prediction of the mechanical properties of the composite. For coupling of the textile reinforcement to the matrix the MSP technique was used. It was implemented in LSDyna by using of the *CONSTRAINED_MULTIPLE_GLOBAL keyword and placing the nodes of the textile mesh as first in the assignment. The same keyword was used to apply the dirichlet periodical BC to the matrix faces. Simulations for all six load cases with implicit iterative solver were performed and then homogenized mechanical properties were compared with experimental in the Table 1. Maximal error lies below 4%. Mechanical property Experiment Simulation Error E x, GPa 37,7 ±,55 36,72,7% E y, GPa 1,5 ±,2 1,9 3,8% G xy, GPa  3,7 µ xy,25,33 µ yx,87,1 Table 1: Mechanical properties of the composite based on lenowoven UD NCF. 5.3 Drapeability Described in Section 4.1 RVE of lenowoven NCF was used to perform the drapeability simulation (Figure 12). Due to the symmetry only one fourth of the model was built with the textile diameter of 33 mm.
9 Fig.12: Model for the draping simulation. In considered test, the punch drives until 8 mm into the fabric from underneath and at steps of 1 mm the force of the punch is taken as well as the pictures of textile on several positions. Total punch force calculated within simulation shows very good agreement with test results (Figure 13). Fig.13: Punch force versus punch displacement obtained from simulation and experiment. The pictures of the textile structure at the highest punch location are compared in the Figure 14. Both experiment and simulation are showing very small amount of gaps at and 45 whereas at 9 the DRAPETEST shows more local gaps which are not observed in simulation results.
10 c) d) e) f) Fig.14: Textile pictures taken from the DRAPETEST camera at the punch displacement 8 mm on a), b) 45 and c) 9 and at the corresponding positions from simulation d f. The contour of the textile after draping made with the camera on the top of the DRAPETEST has very good agreement with the simulation results (Figure 15). Fig.15: Textile shape after draping: a) DRAPETEST and b) simulation.
11 6 Summary In the present work a novel approach for modelling of the reinforcement NCFs was proposed. For estimating of the mechanical behaviour of the textile yarns the microscopic simulations of the roving with different levels of filament misalignments were performed. Obtained properties were direct transferred in the developed user material model and without any parameter tuning very good agreement with experimental results of simple roving compaction was reached both for compression force and crosssection shape change. This material model was also used for generating of the RVE using thermal expansion method of glass lenowoven NCF for different scales of refinement. The drapeability of the textile structure was validated based on drapeability tester called DRAPETEST by Textechno. The forming force converges very well with the measured experimentally. Also the deformation of the textile has the same character. This model may be useful also in simulations of other forming processes like RTM, where the crosssection changes may be significant. MSP method for calculation of the mechanical properties of textile reinforcement composite was implemented in LS Dyna. This method gave the error below 4% comparing to the experimental results. 7 Literature [1] Sherburn M., Geometric and Mechanical Modelling of Textiles, PhD thesis, 27 [2] Lomov S.V., Ivanov D.S., Verpoest I., Zako M., Kurashiki T., Nakai H., Hirosawa S., "MesoFE modelling of textile composites: Road map, data flow and algorithms," Composites Science and Technology, no. 67, pp , 27. [3] Tabatabaei S.A., Lomov S.V., Verpoest I., "Assesment of embedded element technique in mesofe modelling of fibre reinforced composites," Composite structures, no. 17, pp , 214. [4] Jiang WG, Hallett SR, Wisnom M., "Development of domain superposition technique for the modelling of woven fabric composites," in Mechanical response of composites.: Springer, 28. [5] [6] O. Vorobiov: "Interfacing GeoDict Analytical Data to LSDyna and ANSYS", GeoDict User Meeting 214, Kaiserslautern, 214
EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationMESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE
MESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE S. Daggumati a*,i. De Baere a, W. Van Paepegem a, J. Degrieck a, J. Xu b, S.V. Lomov b, I. Verpoest b a Ghent University, Dept. of
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationMULTISCALE MODELLING OF FIBRE BUNDLES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MULTISCALE MODELLING OF FIBRE BUNDLES N. D. Chakladar 1, P. Mandal 1 *, P. Potluri 2 1 School of Mechanical, Aerospace and Civil Engineering,
More informationINVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT
INVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT Andreas Endruweit, Dhiren K. Modi and Andrew C. Long School of Mechanical, Materials and Manufacturing Engineering, University of
More informationAn overview of Carbon Fiber modeling in LSDYNA. John Zhao October 23 th 2017
An overview of Carbon Fiber modeling in LSDYNA John Zhao zhao@lstc.com October 23 th 2017 Outline Manufacturing of Carbon Fiber Compression molding *MAT_277 & 278 *MAT_293 *MAT_249 Resin transform molding
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationNormalisation Of Shear Test Data For Rate Independent Compressible Fabrics
Normalisation Of Shear Test Data For Rate Independent Compressible Fabrics Philip Harrison* 1, Jo Wiggers 2, Andrew C. Long 2 1 University of Glasgow  Room 09 James Watt (South) Building, Materials Engineering
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationMesoscale Modeling of Static and Fatigue Damage in Woven Composite Materials with Finite Element Method
Mesoscale Modeling of Static and Fatigue Damage in Woven Composite Materials with Finite Element Method J. Xu a*, SV. Lomov a, I. Verpoest a, S. Daggumati b, W. Van Paepegem b, J. Degrieck b a Katholieke
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationMeasurement of mesoscale deformations for modelling textile composites
CompTest 2004 Measurement of mesoscale deformations for modelling textile composites P Potluri, D A Perez Ciurezu, R Ramgulam Textile Composites Group University of Manchester Institute of Science & Technology
More informationModelling and numerical simulation of the wrinkling evolution for thermomechanical loading cases
Modelling and numerical simulation of the wrinkling evolution for thermomechanical loading cases Georg Haasemann Conrad Kloß 1 AIMCAL Conference 2016 MOTIVATION Wrinkles in web handling system Loss of
More informationExample 3.7 Consider the undeformed configuration of a solid as shown in Figure 3.60.
162 3. The linear 3D elasticity mathematical model The 3D elasticity model is of great importance, since it is our highest order hierarchical model assuming linear elastic behavior. Therefore, it provides
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationStructural Analysis I Chapter 4  Torsion TORSION
ORSION orsional stress results from the action of torsional or twisting moments acting about the longitudinal axis of a shaft. he effect of the application of a torsional moment, combined with appropriate
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationMODELLING OF DAMAGE IN TEXTILE REINFORCED COMPOSITES: MICRO MESO APPROACH
B. Van Den Broucke et.al., Modelling of damage in textile reinforced composites: micro meso approach MODELLING OF DAMAGE IN TEXTILE REINFORCED COMPOSITES: MICRO MESO APPROACH B. Van Den Broucke,2,, P.
More informationModelling of the bullet perforation of textile targets
Structures Under Shock and Impact IX 355 Modelling of the bullet perforation of textile targets R. Barauskas 1, A. Abraitiene 2 & A. Vilkauskas 1 1 Department of System Analysis, Kaunas University of Technology,
More informationComposites Science and Technology
Composites Science and Technology 7 (1) 194 1941 Contents lists available at ScienceDirect Composites Science and Technology journal homepage: www.elsevier.com/locate/compscitech Local damage in a 5harness
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationPREDICTING THE CONSTITUTIVE BEHAVIOR OF BIAXIAL BRAIDED COMPOSITES USING BEAM UNIT CELLS
THE 19TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PREDICTING THE CONSTITUTIVE BEHAVIOR OF BIAXIAL 1 J. Cichosz1*, J. Bückle1, R. Hinterhölzl1, M. Wolfahrt2 Institute for Carbon Composites, Technische
More informationReview Lecture. AE1108II: Aerospace Mechanics of Materials. Dr. Calvin Rans Dr. Sofia Teixeira De Freitas
Review Lecture AE1108II: Aerospace Mechanics of Materials Dr. Calvin Rans Dr. Sofia Teixeira De Freitas Aerospace Structures & Materials Faculty of Aerospace Engineering Analysis of an Engineering System
More informationUnit 15 Shearing and Torsion (and Bending) of Shell Beams
Unit 15 Shearing and Torsion (and Bending) of Shell Beams Readings: Rivello Ch. 9, section 8.7 (again), section 7.6 T & G 126, 127 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationIDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More informationLocal Strain In A 5  Harness Satin Weave Composite Under Static Tension: Part Ii  MesoFe Analysis
Local Strain In A 5  Harness Satin Weave Composite Under Static Tension: Part Ii  MesoFe Analysis S. Daggumati, W. Van Paepegem, J. Degrieck, T. Praet, B. Verhegghe, J. Xu, S.V. Lomov, I. Verpoest To
More informationINDUSTRIAL FORMING SIMULATION OF MULTILAYERED UD NONCRIMPFABRICS. 13. LSDYNA FORUM, , BAMBERG.
Sebastian Kreissl, Thomas Senner, Arnulf Lipp, Josef Meinhardt. INDUSTRIAL FORMING SIMULATION OF MULTILAYERED UD NONCRIMPFABRICS. 13. LSDYNA FORUM, 07.10.2014, BAMBERG. OUTLINE. BMW i. Production Process
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationBENCHMARK LINEAR FINITE ELEMENT ANALYSIS OF LATERALLY LOADED SINGLE PILE USING OPENSEES & COMPARISON WITH ANALYTICAL SOLUTION
BENCHMARK LINEAR FINITE ELEMENT ANALYSIS OF LATERALLY LOADED SINGLE PILE USING OPENSEES & COMPARISON WITH ANALYTICAL SOLUTION Ahmed Elgamal and Jinchi Lu October 07 Introduction In this study: I) The response
More informationUnit 18 Other Issues In Buckling/Structural Instability
Unit 18 Other Issues In Buckling/Structural Instability Readings: Rivello Timoshenko Jones 14.3, 14.5, 14.6, 14.7 (read these at least, others at your leisure ) Ch. 15, Ch. 16 Theory of Elastic Stability
More informationHomework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. Fall 2004
Homework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. 1. A beam is loaded as shown. The dimensions of the cross section appear in the insert. the figure. Draw a complete free body diagram showing an equivalent
More informationMembers Subjected to Torsional Loads
Members Subjected to Torsional Loads Torsion of circular shafts Definition of Torsion: Consider a shaft rigidly clamped at one end and twisted at the other end by a torque T = F.d applied in a plane perpendicular
More informationREPORT TO DFLEX LTD APRIL 2009 REPORT. (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009)
REPORT (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009) Finite Element Modelling of Rigidity of Fishing Rods with Various Crosssections Report to DFlex Ltd by Z Guan Department of Engineering,
More informationA FULLY COUPLED MULTISCALE SHELL FORMULATION FOR THE MODELLING OF FIBRE REINFORCED LAMINATES
ECCM6 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 24 A FULLY COUPLED MULTISCALE SHELL FORMULATION FOR THE MODELLING OF FIBRE REINFORCED LAMINATES J. Främby, J. Brouzoulis,
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationHomogenization on MultiMaterials Elements: Application to Printed Circuit Boards and Warpage Analysis
Homogenization on MultiMaterials Elements: Application to Printed Circuit Boards and Warpage Analysis Manuel Araújo 1,a, J. L. Alves 1, Paulo Silva 1 and Pedro Delgado 2 1 MEMS, University of Minho, Dep.
More informationSTOCHASTIC MULTISCALE MODELLING OF SHORT AND LONGRANGE EFFECTS IN TEXTILE COMPOSITES BASED ON EXPERIMENTAL DATA
STOCHASTIC MULTISCALE MODELLING OF SHORT AND LONGRANGE EFFECTS IN TEXTILE COMPOSITES BASED ON EXPERIMENTAL DATA A. Vanaerschot 1, B. N. Cox 2, S. V. Lomov 3, D. Vandepitte 1 1 KU Leuven, Dept. of Mechanical
More informationApplication of Finite Element Method to Create Animated Simulation of Beam Analysis for the Course of Mechanics of Materials
International Conference on Engineering Education and Research "Progress Through Partnership" 4 VSBTUO, Ostrava, ISSN 15635 Application of Finite Element Method to Create Animated Simulation of Beam
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationUsing the finite element method of structural analysis, determine displacements at nodes 1 and 2.
Question 1 A pinjointed plane frame, shown in Figure Q1, is fixed to rigid supports at nodes and 4 to prevent their nodal displacements. The frame is loaded at nodes 1 and by a horizontal and a vertical
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationSHEAR TENSION COUPLING IN BIAXIAL BIAS EXTENSION TESTS
SHER TENSION COUPLING IN IXIL IS EXTENSION TESTS P. Harrison *, P. Potluri Department of Mechanical Engineering, James Watt uilding (South), University of Glasgow, Glasgow G 8QQ, U.K. p.harrison@mech.gla.ac.uk
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationNomenclature. Length of the panel between the supports. Width of the panel between the supports/ width of the beam
omenclature a b c f h Length of the panel between the supports Width of the panel between the supports/ width of the beam Sandwich beam/ panel core thickness Thickness of the panel face sheet Sandwich
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationIntroduction, Basic Mechanics 2
Computational Biomechanics 18 Lecture : Introduction, Basic Mechanics Ulli Simon, Lucas Engelhardt, Martin Pietsch Scientific Computing Centre Ulm, UZWR Ulm University Contents Mechanical Basics Moment
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationCOMPOSITE REINFORCEMENT FORMING SIMULATION: A MULTISCALE APPROACH
COMPOSITE REINFORCEMENT FORMING SIMULATION: A MULTISCALE APPROACH N. Hamila A. Khan S. Gatouillat E. De Luycker E. VidalSallé T. Mabrouki P. Boisse Université de Lyon, LaMCoS, INSALyon Philippe.Boisse@insalyon.fr
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationEffects of mesostructure on the inplane properties of tufted carbon fabric composites
Effects of mesostructure on the inplane properties of tufted carbon fabric composites CompTest 2011, 14 th February 2011 Johannes W G Treiber Denis D R Cartié Ivana K Partridge j.treiber@cranfield.ac.uk
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationFinite Element Static, Vibration and ImpactContact Analysis of Micromechanical Systems
Finite Element Static, Vibration and ImpactContact Analysis of Micromechanical Systems Alexey I. Borovkov Eugeny V. Pereyaslavets Igor A. Artamonov Computational Mechanics Laboratory, St.Petersburg State
More informationFurther Linear Elasticity
Torsion of cylindrical bodies Further Linear Elasticity Problem Sheet # 1. Consider a cylindrical body of length L, the ends of which are subjected to distributions of tractions that are statically equivalent
More informationModule 2 Stresses in machine elements. Version 2 ME, IIT Kharagpur
Module Stresses in machine elements Lesson Compound stresses in machine parts Instructional Objectives t the end of this lesson, the student should be able to understand Elements of force system at a beam
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationArbitrary Normal and Tangential Loading Sequences for Circular Hertzian Contact
Arbitrary Normal and Tangential Loading Sequences for Circular Hertzian Contact Philip P. Garland 1 and Robert J. Rogers 2 1 School of Biomedical Engineering, Dalhousie University, Canada 2 Department
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationTheoretical Manual Theoretical background to the Strand7 finite element analysis system
Theoretical Manual Theoretical background to the Strand7 finite element analysis system Edition 1 January 2005 Strand7 Release 2.3 20042005 Strand7 Pty Limited All rights reserved Contents Preface Chapter
More informationContent. Department of Mathematics University of Oslo
Chapter: 1 MEK4560 The Finite Element Method in Solid Mechanics II (January 25, 2008) (Epost:torgeiru@math.uio.no) Page 1 of 14 Content 1 Introduction to MEK4560 3 1.1 Minimum Potential energy..............................
More informationMechanics of Materials II. Chapter III. A review of the fundamental formulation of stress, strain, and deflection
Mechanics of Materials II Chapter III A review of the fundamental formulation of stress, strain, and deflection Outline Introduction Assumtions and limitations Axial loading Torsion of circular shafts
More informationStructural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian
Structural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian ahmadian@iust.ac.ir Dynamic Response of MDOF Systems: ModeSuperposition Method ModeSuperposition Method:
More informationFINITE ELEMENT ANALYSIS OF ARKANSAS TEST SERIES PILE #2 USING OPENSEES (WITH LPILE COMPARISON)
FINITE ELEMENT ANALYSIS OF ARKANSAS TEST SERIES PILE #2 USING OPENSEES (WITH LPILE COMPARISON) Ahmed Elgamal and Jinchi Lu October 07 Introduction In this study, we conduct a finite element simulation
More informationModeling nonisothermal thermoforming of fabricreinforced thermoplastic composites
Modeling nonisothermal thermoforming of fabricreinforced thermoplastic composites Dominic Schommer, Miro Duhovic, Joachim Hausmann Institut für Verbundwerkstoffe GmbH, ErwinSchrödingerStr., Building
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationNUMERICAL DESIGN OF COMPOSITE MATERIALS THROUGH MULTISCALE COMPUTER SIMULATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS NUMERICAL DESIGN OF COMPOSITE MATERIALS THROUGH J. Leach 1 *, J. Mackiewicz 2, Dr. S. Risser 1 1 Battelle Memorial Institute, Columbus, OH, USA,
More information46th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference April 2005 Austin, Texas
th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference  April, Austin, Texas AIAA  AIAA  Bistable Cylindrical Space Frames H Ye and S Pellegrino University of Cambridge, Cambridge,
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationMATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS
. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stressstrain
More informationFLEXIBILITY METHOD FOR INDETERMINATE FRAMES
UNIT  I FLEXIBILITY METHOD FOR INDETERMINATE FRAMES 1. What is meant by indeterminate structures? Structures that do not satisfy the conditions of equilibrium are called indeterminate structure. These
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationProblem " Â F y = 0. ) R A + 2R B + R C = 200 kn ) 2R A + 2R B = 200 kn [using symmetry R A = R C ] ) R A + R B = 100 kn
Problem 0. Three cables are attached as shown. Determine the reactions in the supports. Assume R B as redundant. Also, L AD L CD cos 60 m m. uation of uilibrium: + " Â F y 0 ) R A cos 60 + R B + R C cos
More informationA numerical parametric study on the plate inclination angle of steel plate shear walls
Journal of Structural Engineering & Applied Mechanics 219 Volume 1 Issue 4 164173 https://doi.org/1.31462/jseam.219.1164173 www.goldenlightpublish.com RESEARCH ARTICLE A numerical parametric study on
More information[7] Torsion. [7.1] Torsion. [7.2] Statically Indeterminate Torsion. [7] Torsion Page 1 of 21
[7] Torsion Page 1 of 21 [7] Torsion [7.1] Torsion [7.2] Statically Indeterminate Torsion [7] Torsion Page 2 of 21 [7.1] Torsion SHEAR STRAIN DUE TO TORSION 1) A shaft with a circular cross section is
More informationMECHANICS OF MATERIALS
STATICS AND MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr, John T. DeWolf David E Mazurek \Cawect Mc / iur/» Craw SugomcT Hilt Introduction 1 1.1 What is Mechanics? 2 1.2 Fundamental
More informationY. M. TEMIS AND V. V. KARABAN 1
J. KSIAM Vol.5, No.2, 3951, 2001 BOUNDARY ELEMENT TECHNIQUE IN TORSION PROBLEMS OF BEAMS WITH MULTIPLY CONNECTED CROSSSECTIONS Y. M. TEMIS AND V. V. KARABAN 1 Abstract. This paper shows how boundary
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationThe stiffness of plates
The stiffness of plates 1. Introduction The word plate is a collective term for elements in which forces can be transferred in two directions. Floors, walls, bridge slabs and laminates are all plates.
More informationTEXTILE IMPREGNATION WITH THERMOPLASTIC RESIN MODELS AND APPLICATION
TEXTILE IMPREGNATION WITH THERMOPLASTIC RESIN MODELS AND APPLICATION Richard Loendersloot 1, Wouter Grouve 2, Edwin Lamers 3 and Sebastiaan Wijskamp 4 1 Applied Mechanics, University of Twente, P.O. Box
More information